LMucko/crystallography-open-database huggingface dataset:
Direct and indirect preparation of layered quaternary manganese tellurides; A Mnx My Te2 (A= Li, Na; M= Cu, Ag; x+y<= 2)
Kim, J.; Hughbanks, T.; Journal of Alloys Compd. 327 (2001) 116–120; doi:

data_1526622
_publ_section_title
;
 Direct and indirect preparation of layered quaternary manganese
 tellurides; A Mnx My Te2 (A= Li, Na; M= Cu, Ag; x+y<= 2)
;
_journal_name_full               'Journal of Alloys Compd.'
_journal_page_first              116
_journal_page_last               120
_journal_volume                  327
_journal_year                    2001
_chemical_formula_sum            'Cu0.19 Li Mn0.98 Te2'
_chemical_name_systematic        'Li Mn0.98 Cu0.19 Te2'
_space_group_IT_number           164
_symmetry_space_group_name_Hall  '-P 3 2"'
_symmetry_space_group_name_H-M   'P -3 m 1'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            1
_cell_length_a                   4.478
_cell_length_b                   4.478
_cell_length_c                   7.17
_cell_volume                     124.514
_citation_journal_id_ASTM        JALCEU
_cod_data_source_file            Kim_JALCEU_2001_1323.cif
_cod_data_source_block           Cu0.19Li1Mn0.98Te2
_cod_original_cell_volume        124.5139
_cod_original_formula_sum        'Cu0.19 Li1 Mn0.98 Te2'
_cod_database_code               1526622
The crystal chemistry of superconducting Sr3.66 Bi0.28 Ca6.02 Cu16.45 O28.63 and nonsuperconducting Sr5.97 Ca3.13 Y0.53 Al0.25 Bi0.12 Cu16.66 O28.64 compounds
Shvanskaya, L.; Sokolova, E.; Leonyuk, L.; Maltsev, V.; Zeitschrift fuer Kristallographie (149,1979-) 215 (2000) 368–372; doi:

data_8103631
_publ_section_title
;
 The crystal chemistry of superconducting Sr3.66 Bi0.28 Ca6.02 Cu16.45
 O28.63 and nonsuperconducting Sr5.97 Ca3.13 Y0.53 Al0.25 Bi0.12 Cu16.66
 O28.64 compounds
;
_journal_name_full
'Zeitschrift fuer Kristallographie (149,1979-)'
_journal_page_first              368
_journal_page_last               372
_journal_volume                  215
_journal_year                    2000
_chemical_formula_sum
'Al0.26 Bi0.12 Ca3.128 Cu16.537 O28.476 Sr5.964 Y0.534'
_chemical_name_systematic
;
Bi0.12 Al0.26 Y0.534 Ca3.128 Sr5.964 Cu16.537 O28.476
;
_space_group_IT_number           22
_symmetry_space_group_name_Hall  'F 2 2'
_symmetry_space_group_name_H-M   'F 2 2 2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   11.346
_cell_length_b                   12.996
_cell_length_c                   19.585
_cell_volume                     2887.859
_citation_journal_id_ASTM        ZEKRDZ
_cod_data_source_file            Shvanskaya_ZEKRDZ_2000_812.cif
_cod_data_source_block           Al0.26Bi0.12Ca3.128Cu16.537O28.476Sr5.964Y0.534
_cod_database_code               8103631
Direct and indirect preparation of layered quaternary manganese tellurides; A Mnx My Te2 (A = Li, Na; M = Cu, Ag; x+y<=2)
Kim, J.; Hughbanks, T.; Journal of Alloys Compd. 327 (2001) 116–120; doi:

data_1526623
_publ_section_title
;
 Direct and indirect preparation of layered quaternary manganese
 tellurides; A Mnx My Te2 (A = Li, Na; M = Cu, Ag; x+y<=2)
;
_journal_name_full               'Journal of Alloys Compd.'
_journal_page_first              116
_journal_page_last               120
_journal_volume                  327
_journal_year                    2001
_chemical_formula_sum            'Cu0.98 Mn1.01 Na0.91 Te2'
_chemical_name_systematic        'Na0.91 Mn1.01 Cu0.98 Te2'
_space_group_IT_number           164
_symmetry_space_group_name_Hall  '-P 3 2"'
_symmetry_space_group_name_H-M   'P -3 m 1'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            1
_cell_length_a                   4.4901
_cell_length_b                   4.4901
_cell_length_c                   7.5364
_cell_volume                     131.585
_citation_journal_id_ASTM        JALCEU
_cod_data_source_file            Kim_JALCEU_2001_1324.cif
_cod_data_source_block           Cu0.98Mn1.01Na0.91Te2
_cod_original_cell_volume        131.5851
_cod_database_code               1526623
The crystal chemistry of superconducting Sr3.66 Bi0.28 Ca6.02 Cu16.45 O28.63 and nonsuperconducting Sr5.97 Ca3.13 Y0.53 Al0.25 Bi0.12 Cu16.66 O28.64 compounds
Shvanskaya, L.; Leonyuk, L.; Sokolova, E.; Maltsev, V.; Zeitschrift fuer Kristallographie (149,1979-) 215 (2000) 368–372; doi:

data_8103632
_publ_section_title
;
 The crystal chemistry of superconducting Sr3.66 Bi0.28 Ca6.02 Cu16.45
 O28.63 and nonsuperconducting Sr5.97 Ca3.13 Y0.53 Al0.25 Bi0.12 Cu16.66
 O28.64 compounds
;
_journal_name_full
'Zeitschrift fuer Kristallographie (149,1979-)'
_journal_page_first              368
_journal_page_last               372
_journal_volume                  215
_journal_year                    2000
_chemical_formula_sum            'Bi0.28 Ca6.024 Cu16.447 O28.63 Sr3.66'
_chemical_name_systematic        'Bi0.28 Sr3.66 Ca6.024 Cu16.447 O28.63'
_space_group_IT_number           22
_symmetry_space_group_name_Hall  'F 2 2'
_symmetry_space_group_name_H-M   'F 2 2 2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   11.319
_cell_length_b                   12.763
_cell_length_c                   19.491
_cell_volume                     2815.756
_citation_journal_id_ASTM        ZEKRDZ
_cod_data_source_file            Shvanskaya_ZEKRDZ_2000_813.cif
_cod_data_source_block           Bi0.28Ca6.024Cu16.447O28.63Sr3.66
_cod_original_cell_volume        2815.755
_cod_database_code               8103632
Crystal structure and phase transitions of Sr1+x Bi2+y Ta2 O9 ceramics
Kim, J.S.; Cheon, C.-I.; Shim, H.-S.; Lee, C.H.; Journal of the European Ceramic Society 21 (2001) 1295–1298; doi:

data_1526624
_publ_section_title
;
 Crystal structure and phase transitions of Sr1+x Bi2+y Ta2 O9 ceramics
;
_journal_name_full               'Journal of the European Ceramic Society'
_journal_page_first              1295
_journal_page_last               1298
_journal_volume                  21
_journal_year                    2001
_chemical_formula_sum            'Bi2.01 O9 Sr0.9 Ta2'
_chemical_name_systematic        '(Sr0.9 Bi0.09) Bi1.92 Ta2 O9'
_space_group_IT_number           36
_symmetry_space_group_name_Hall  'A -2 2a'
_symmetry_space_group_name_H-M   'A 21 a m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   5.522
_cell_length_b                   5.524
_cell_length_c                   25.026
_cell_volume                     763.381
_citation_journal_id_ASTM        JECSER
_cod_data_source_file            Kim_JECSER_2001_1487.cif
_cod_data_source_block           Bi2.01O9Sr0.9Ta2
_cod_original_cell_volume        763.3813
_cod_original_sg_symbol_Hall     'C 2c -2 (z,y,-x)'
_cod_database_code               1526624
Pr4 S3 (Si2 O7) und Pr3 Cl3 (Si2 O7) : durch weiche Fremdanionen modifizierte Derivate von Praseodymsilicat
Sieke, C.; Schleid, T.; Zeitschrift fuer Anorganische und Allgemeine Chemie 626 (2000) 196–201; doi:

data_1526625
_publ_section_title
;
 Pr4 S3 (Si2 O7) und Pr3 Cl3 (Si2 O7) : durch weiche Fremdanionen
 modifizierte Derivate von Praseodymsilicat
;
_journal_name_full
'Zeitschrift fuer Anorganische und Allgemeine Chemie'
_journal_page_first              196
_journal_page_last               201
_journal_volume                  626
_journal_year                    2000
_chemical_formula_sum            'O7 Pr4 S3 Si2'
_chemical_name_systematic        'Pr4 S3 (Si2 O7)'
_space_group_IT_number           141
_symmetry_space_group_name_Hall  '-I 4bd 2'
_symmetry_space_group_name_H-M   'I 41/a m d :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   12.016
_cell_length_b                   12.016
_cell_length_c                   14.12
_cell_volume                     2038.706
_citation_journal_id_ASTM        ZAACAB
_cod_data_source_file            Sieke_ZAACAB_2000_762.cif
_cod_data_source_block           O7Pr4S3Si2
_cod_database_code               1526625
Crystal structure and phase transitions of Sr1+x Bi2+y Ta2 O9 ceramics
Kim, J.S.; Cheon, C.-I.; Shim, H.-S.; Lee, C.H.; Journal of the European Ceramic Society 21 (2001) 1295–1298; doi:

data_1526626
_publ_section_title
;
 Crystal structure and phase transitions of Sr1+x Bi2+y Ta2 O9 ceramics
;
_journal_name_full               'Journal of the European Ceramic Society'
_journal_page_first              1295
_journal_page_last               1298
_journal_volume                  21
_journal_year                    2001
_chemical_formula_sum            'Bi2 O9 Sr Ta2'
_chemical_name_systematic        'Sr Bi2 (Ta2 O9)'
_space_group_IT_number           41
_symmetry_space_group_name_Hall  'A 2 -2ab'
_symmetry_space_group_name_H-M   'A b a 2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   5.533
_cell_length_b                   25.125
_cell_length_c                   5.534
_cell_volume                     769.318
_citation_journal_id_ASTM        JECSER
_cod_data_source_file            Kim_JECSER_2001_1488.cif
_cod_data_source_block           Bi2O9Sr1Ta2
_cod_original_formula_sum        'Bi2 O9 Sr1 Ta2'
_cod_database_code               1526626
Pr4 S3 (Si2 O7) und Pr3 Cl3 (Si2 O7) : durch weiche Fremdanionen modifizierte Derivate von Praseodymsilicat
Sieke, C.; Schleid, T.; Zeitschrift fuer Anorganische und Allgemeine Chemie 626 (2000) 196–201; doi:

data_1526627
_publ_section_title
;
 Pr4 S3 (Si2 O7) und Pr3 Cl3 (Si2 O7) : durch weiche Fremdanionen
 modifizierte Derivate von Praseodymsilicat
;
_journal_name_full
'Zeitschrift fuer Anorganische und Allgemeine Chemie'
_journal_page_first              196
_journal_page_last               201
_journal_volume                  626
_journal_year                    2000
_chemical_formula_sum            'Cl3 O7 Pr3 Si2'
_chemical_name_systematic        'Pr3 Cl3 (Si2 O7)'
_space_group_IT_number           4
_symmetry_space_group_name_Hall  'P 2yb'
_symmetry_space_group_name_H-M   'P 1 21 1'
_cell_angle_alpha                90
_cell_angle_beta                 109.07
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   5.3096
_cell_length_b                   12.002
_cell_length_c                   7.8311
_cell_volume                     471.656
_citation_journal_id_ASTM        ZAACAB
_cod_data_source_file            Sieke_ZAACAB_2000_763.cif
_cod_data_source_block           Cl3O7Pr3Si2
_cod_original_cell_volume        471.6558
_cod_database_code               1526627
Synthesis of Ba0.6 K0.4 Bi O3 superconductors and structural analysis using neutron powder diffraction
Kim, H.-T.; Kang, K.-Y.; Choi, Y.-N.; Kim, W.-J.; Kim, B.J.; Kim, Y.C.; Journal of the Korean Physical Society 39 (2001) 1013–1018; doi:

data_1526628
_publ_section_title
;
 Synthesis of Ba0.6 K0.4 Bi O3 superconductors and structural analysis
 using neutron powder diffraction
;
_journal_name_full               'Journal of the Korean Physical Society'
_journal_page_first              1013
_journal_page_last               1018
_journal_volume                  39
_journal_year                    2001
_chemical_formula_sum            'Ba0.6 Bi K0.4 O3'
_chemical_name_systematic        '(Ba0.6 K0.4) (Bi O3)'
_space_group_IT_number           221
_symmetry_space_group_name_Hall  '-P 4 2 3'
_symmetry_space_group_name_H-M   'P m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            1
_cell_length_a                   4.27841
_cell_length_b                   4.27841
_cell_length_c                   4.27841
_cell_volume                     78.315
_citation_journal_id_ASTM        JKPSDV
_cod_data_source_file            Kim_JKPSDV_2001_1799.cif
_cod_data_source_block           Ba0.6Bi1K0.4O3
_cod_original_cell_volume        78.31541
_cod_original_formula_sum        'Ba0.6 Bi1 K0.4 O3'
_cod_database_code               1526628
Zur Dimorphie von Nd3 Cl (Si O4)2
Sieke, C.; Hartenbach, I.; Schleid, T.; Zeitschrift fuer Anorganische und Allgemeine Chemie 626 (2000) 2236–2239; doi:

data_1526629
_publ_section_title
;
 Zur Dimorphie von Nd3 Cl (Si O4)2
;
_journal_name_full
'Zeitschrift fuer Anorganische und Allgemeine Chemie'
_journal_page_first              2236
_journal_page_last               2239
_journal_volume                  626
_journal_year                    2000
_chemical_formula_sum            'Cl Nd3 O8 Si2'
_chemical_name_systematic        'Nd3 Cl (Si O4)2'
_space_group_IT_number           15
_symmetry_space_group_name_Hall  '-C 2yc'
_symmetry_space_group_name_H-M   'C 1 2/c 1'
_cell_angle_alpha                90
_cell_angle_beta                 98.403
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   14.166
_cell_length_b                   6.3879
_cell_length_c                   8.7221
_cell_volume                     780.798
_citation_journal_id_ASTM        ZAACAB
_cod_data_source_file            Sieke_ZAACAB_2000_779.cif
_cod_data_source_block           Cl1Nd3O8Si2
_cod_original_cell_volume        780.7984
_cod_original_formula_sum        'Cl1 Nd3 O8 Si2'
_cod_database_code               1526629
Zur Dimorphie von Nd3 Cl (Si O4)2
Sieke, C.; Hartenbach, I.; Schleid, T.; Zeitschrift fuer Anorganische und Allgemeine Chemie 626 (2000) 2236–2239; doi:

data_1526630
_publ_section_title
;
 Zur Dimorphie von Nd3 Cl (Si O4)2
;
_journal_name_full
'Zeitschrift fuer Anorganische und Allgemeine Chemie'
_journal_page_first              2236
_journal_page_last               2239
_journal_volume                  626
_journal_year                    2000
_chemical_formula_sum            'Cl Nd3 O8 Si2'
_chemical_name_systematic        'Nd3 Cl (Si O4)2'
_space_group_IT_number           62
_symmetry_space_group_name_Hall  '-P 2ac 2n'
_symmetry_space_group_name_H-M   'P n m a'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   7.0936
_cell_length_b                   18.157
_cell_length_c                   6.3148
_cell_volume                     813.337
_citation_journal_id_ASTM        ZAACAB
_cod_data_source_file            Sieke_ZAACAB_2000_780.cif
_cod_data_source_block           Cl1Nd3O8Si2
_cod_original_cell_volume        813.3367
_cod_original_formula_sum        'Cl1 Nd3 O8 Si2'
_cod_database_code               1526630
Cubic aluminium silicides RE8 Ru12 Al49 Si9 (Alx Si12-x) (RE = Pr, Sm) from liquid aluminum. Empty (Si, Al)12 cuboctahedral clusters and assignment of the Al/Si distribution with neutron diffraction
Sieve, B.; Henning, R.; Chen, X.Z.; Kanatzidis, M.G.; Kannewurf, C.R.; Brazis, P.; Schultz, A.J.; Cowen, J.A.; Journal of the American Chemical Society 123 (2001) 7040–7047; doi:

data_4123967
_publ_section_title
;
 Cubic aluminium silicides RE8 Ru12 Al49 Si9 (Alx Si12-x) (RE = Pr, Sm)
 from liquid aluminum. Empty (Si, Al)12 cuboctahedral clusters and
 assignment of the Al/Si distribution with neutron diffraction
;
_journal_name_full               'Journal of the American Chemical Society'
_journal_page_first              7040
_journal_page_last               7047
_journal_volume                  123
_journal_year                    2001
_chemical_formula_sum            'Al52.996 Ru12 Si17.004 Sm8'
_chemical_name_systematic        'Sm8 Ru12 Al49 Si9 (Al0.333 Si0.667)12'
_space_group_IT_number           221
_symmetry_space_group_name_Hall  '-P 4 2 3'
_symmetry_space_group_name_H-M   'P m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            1
_cell_length_a                   11.5101
_cell_length_b                   11.5101
_cell_length_c                   11.5101
_cell_volume                     1524.886
_citation_journal_id_ASTM        JACSAT
_cod_data_source_file            Sieve_JACSAT_2001_1118.cif
_cod_data_source_block           Al52.996Ru12Si17.004Sm8
_cod_database_code               4123967
High pressure synthesis and crystal structure of a new Ni(III) perovskite: Tl Ni O3
Kim, S.-J.; Demazeau, G.; Alonso, J.A.; Choy, J.-H.; Journal of Materials Chemistry 11 (2001) 487–492; doi:

data_7221317
_publ_section_title
;
 High pressure synthesis and crystal structure of a new Ni(III)
 perovskite: Tl Ni O3
;
_journal_name_full               'Journal of Materials Chemistry'
_journal_page_first              487
_journal_page_last               492
_journal_volume                  11
_journal_year                    2001
_chemical_formula_sum            'Ni O3 Tl'
_chemical_name_systematic        'Tl Ni O3'
_space_group_IT_number           62
_symmetry_space_group_name_Hall  '-P 2c 2ab'
_symmetry_space_group_name_H-M   'P b n m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   5.2549
_cell_length_b                   5.3677
_cell_length_c                   7.562
_cell_volume                     213.299
_citation_journal_id_ASTM        JMACEP
_cod_data_source_file            Kim_JMACEP_2001_1406.cif
_cod_data_source_block           Ni1O3Tl1
_cod_original_cell_volume        213.2993
_cod_original_sg_symbol_Hall     '-P 2ac 2n (z,x,y)'
_cod_original_formula_sum        'Ni1 O3 Tl1'
_cod_database_code               7221317
Cubic aluminium silicides RE8 Ru12 Al49 Si9 (Alx Si12-x) (RE= Pr, Sm) from liquid aluminum. Empty (Si, Al)12 cuboctahedral clusters and assignment of the Al/Si distribution with neutron diffraction
Sieve, B.; Chen, X.Z.; Henning, R.; Brazis, P.; Kannewurf, C.R.; Cowen, J.A.; Schultz, A.J.; Kanatzidis, M.G.; Journal of the American Chemical Society 123 (2001) 7040–7047; doi:

data_4123968
_publ_section_title
;
 Cubic aluminium silicides RE8 Ru12 Al49 Si9 (Alx Si12-x) (RE= Pr, Sm)
 from liquid aluminum. Empty (Si, Al)12 cuboctahedral clusters and
 assignment of the Al/Si distribution with neutron diffraction
;
_journal_name_full               'Journal of the American Chemical Society'
_journal_page_first              7040
_journal_page_last               7047
_journal_volume                  123
_journal_year                    2001
_chemical_formula_sum            'Al53.44 Pr8 Ru12 Si16.56'
_chemical_name_systematic        'Pr8 Ru12 Al49 Si9 (Al0.37 Si0.63)12'
_space_group_IT_number           221
_symmetry_space_group_name_Hall  '-P 4 2 3'
_symmetry_space_group_name_H-M   'P m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            1
_cell_length_a                   11.553
_cell_length_b                   11.553
_cell_length_c                   11.553
_cell_volume                     1542.000
_citation_journal_id_ASTM        JACSAT
_cod_data_source_file            Sieve_JACSAT_2001_1119.cif
_cod_data_source_block           Al53.44Pr8Ru12Si16.56
_cod_original_cell_volume        1542
_cod_database_code               4123968
Yb5 In2 Sb6: a new rare earth Zintl phase with a narrow band gap
Kim, S.-J.; Ireland, J.R.; Kanatzidis, M.G.; Kannewurf, C.R.; Journal of Solid State Chemistry 155 (2000) 55–61; doi:

data_1526631
_publ_section_title
;
 Yb5 In2 Sb6: a new rare earth Zintl phase with a narrow band gap
;
_journal_name_full               'Journal of Solid State Chemistry'
_journal_page_first              55
_journal_page_last               61
_journal_volume                  155
_journal_year                    2000
_chemical_formula_sum            'In2 Sb6 Yb5'
_chemical_name_systematic        'Yb5 In2 Sb6'
_space_group_IT_number           55
_symmetry_space_group_name_Hall  '-P 2 2ab'
_symmetry_space_group_name_H-M   'P b a m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   7.3992
_cell_length_b                   23.001
_cell_length_c                   4.5139
_cell_volume                     768.216
_citation_journal_id_ASTM        JSSCBI
_cod_data_source_file            Kim_JSSCBI_2000_77.cif
_cod_data_source_block           In2Sb6Yb5
_cod_original_cell_volume        768.2161
_cod_database_code               1526631
Crystal structure of K4 Pu (S O4)4 * 2(H2 O)
Singh Mudher, K.D.; Krishnan, K.; Journal of Alloys Compd. 313 (2000) 65–68; doi:

data_1526632
_publ_section_title
;
 Crystal structure of K4 Pu (S O4)4 * 2(H2 O)
;
_journal_name_full               'Journal of Alloys Compd.'
_journal_page_first              65
_journal_page_last               68
_journal_volume                  313
_journal_year                    2000
_chemical_formula_sum            'H4 K4 O18 Pu S4'
_chemical_name_systematic        'K4 Pu (S O4)4 (H2 O)2'
_space_group_IT_number           14
_symmetry_space_group_name_Hall  '-P 2ybc'
_symmetry_space_group_name_H-M   'P 1 21/c 1'
_cell_angle_alpha                90
_cell_angle_beta                 111.82
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   12.4175
_cell_length_b                   11.1583
_cell_length_c                   13.553
_cell_volume                     1743.341
_citation_journal_id_ASTM        JALCEU
_cod_data_source_file            SinghMudher_JALCEU_2000_128.cif
_cod_data_source_block           H4K4O18Pu1S4
_cod_original_formula_sum        'H4 K4 O18 Pu1 S4'
_cod_database_code               1526632
Structural distortion and chemical bonding in Tl Fe O3: comparison with A Fe O3 (A = rare earth)
Kim, S.-J.; Choy, J.-H.; Presnyakov, I.A.; Demazeau, G.; Journal of Solid State Chemistry 161 (2001) 197–204; doi:

data_1526633
_publ_section_title
;
 Structural distortion and chemical bonding in Tl Fe O3: comparison with A
 Fe O3 (A = rare earth)
;
_journal_name_full               'Journal of Solid State Chemistry'
_journal_page_first              197
_journal_page_last               204
_journal_volume                  161
_journal_year                    2001
_chemical_formula_sum            'Fe O3 Tl'
_chemical_name_systematic        'Tl (Fe O3)'
_space_group_IT_number           62
_symmetry_space_group_name_Hall  '-P 2c 2ab'
_symmetry_space_group_name_H-M   'P b n m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   5.3172
_cell_length_b                   5.4465
_cell_length_c                   7.7927
_cell_volume                     225.678
_citation_journal_id_ASTM        JSSCBI
_cod_data_source_file            Kim_JSSCBI_2001_1680.cif
_cod_data_source_block           Fe1O3Tl1
_cod_original_cell_volume        225.6776
_cod_original_sg_symbol_Hall     '-P 2ac 2n (z,x,y)'
_cod_original_formula_sum        'Fe1 O3 Tl1'
_cod_database_code               1526633